#------------------------------------------------------------------------------
#$Date: 2014-08-15 21:14:22 +0300 (Fri, 15 Aug 2014) $
#$Revision: 23 $
#$URL: svn+ssh://sauliusg@svn.code.sf.net/p/propcif/code/trunk/cif/1/1000098.mpod $
#------------------------------------------------------------------------------
#
# This file is available in the Material Properties Open Database (MPOD),
# http://www.mpod.net/
#
# The file may be used within the scientific community so long as
# proper attribution is given to the journal article from which the
# data were obtained.
#
data_1000098
_cod_database_code ?
_structure_refined 'yes'
_mpod_phase_name 'Mullite 3:2'
_chemical_formula_sum 'Al5 Si O9.5'
_mpod_symmetry_point_group_name_H-M mmm
_cell_length_a 7.58(1)
_cell_length_b 7.68(1)
_cell_length_c 2.90(1)
loop_
_publ_author_name
'Kriven, W.M.'
'Palko, J.W.'
'Sinogeikin, S.'
'Bass, J.D.'
'Sayir, A.'
'Brunauer, G.'
'Boysen, H.'
'Frey, F.'
'Schneider, J.'
_publ_section_title
;
 High temperature single crystal properties of mullite
;
_journal_name_full               'Journal of the European Ceramic Society'
_journal_volume                  19
_journal_page_first              2529
_journal_page_last               2541
_journal_year                    1999
_mpod_phase_density 3100
_prop_measurement_method 'BS'
_prop_elastic_stiffness_cij 'cij'
loop_
_prop_data_label
_prop_data_tensorial_index
_prop_data_value
cij 11 280
cij 12 105
cij 13 99.2
cij 22 245
cij 23 135
cij 33 362
cij 44 111
cij 55 78.1
cij 66 79.0
